Presentation on theme: "CHAPTER 4 MACROMECHANICAL ANALYSIS OF LAMINATES"— Presentation transcript:
1 CHAPTER 4 MACROMECHANICAL ANALYSIS OF LAMINATES Dr. Ahmet Erkliğ
2 Laminate CodeA laminate is made of a group of single layers bonded to each other. Each layer can be identiﬁed by its location in the laminate, its material, and its angle of orientation with a reference axis.
6 Special Types of Laminates Symmetric laminate: for every ply above the laminate midplane, there is an identical ply (material and orientation) an equal distance below the midplaneBalanced laminate: for every ply at a +θ orientation, there is another ply at the – θ orientation somewhere in the laminateCross-ply laminate: composed of plies of either 0˚ or 90˚ (no other ply orientation)Quansi-isotropic laminate: produced using at least three different ply orientations, all with equal angles between them. Exhibits isotropic extensional stiffness properties
10 Strain-Displacement Equations The classical lamination theory is used to develop these relationships. Assumptions:Each lamina is orthotropic.Each lamina is homogeneous.A line straight and perpendicular to the middle surface remains straight and perpendicular to the middle surface during deformation
11 Strain-Displacement Equations The laminate is thin and is loaded only in its plane (plane stress)Displacements are continuous and small throughout the laminateEach lamina is elasticNo slip occurs between the lamina interfaces
12 Strain-Displacement Equations Nx = normal force resultant in the x direction (per unit length) Ny = normal force resultant in the y direction (per unit length) Nxy = shear force resultant (per unit length)
13 Strain-Displacement Equations Mx = bending moment resultant in the yz plane (per unit length) My = bending moment resultant in the xz plane (per unit length) Mxy = twisting moment resultant (per unit length)
20 Coordinate Locations of Plies in a Laminate Consider a laminate made of n plies. Each ply has a thickness of tk . Then the thickness of the laminate h is
21 Coordinate Locations of Plies in a Laminate The z-coordinate of each ply k surface (top and bottom) is given byPly 1:Ply k: (k = 2, 3,…n – 2, n – 1):Ply n:
22 Integrating the global stresses in each lamina gives the resultant forces per unit length in the x–y plane through the laminate thickness asSimilarly, integrating the global stresses in each lamina gives the resulting moments per unit length in the x–y plane through the laminate thickness as
29 Force and Moment Resultant [A] – extensional stiffness matrix relating the resultant in-plane forces to the in-plane strains.[B] – coupling stiffness matrix coupling the force and moment terms to the midplane strains and midplane curvatures.[D] – bending stiffness matrix relating the resultant bending moments to the plate curvatures.
31 Analysis Procedures for Laminated Composites Find the value of the reduced stiffness matrix [Q] for each ply using its four elastic moduli, E1 , E2 , ν12 , and G12Find the value of the transformed reduced stiffness matrix [ 𝑄 ] for each ply using the [Q] matrix calculated in step 1 and the angle of the plyKnowing the thickness, tk , of each ply, ﬁnd the coordinate of the top and bottom surface, hi , i = 1…, n, of each ply.Use the [ 𝑄 ] matrices from step 2 and the location of each ply from step 3 to ﬁnd the three stiffness matrices [A], [B], and [D]
32 Analysis Procedures for Laminated Composites Substitute the stiffness matrix values found in step 4 and the applied forces and momentsSolve the six simultaneous equations to ﬁnd the midplane strains and curvatures.Now that the location of each ply is known, ﬁnd the global strains in each plyFor ﬁnding the global stresses, use the stress–strainFor ﬁnding the local strains, use the transformationFor ﬁnding the local stresses, use the transformation
33 ExampleFind the three stiffness matrices [A], [B], and [D] for a three-ply [0/30/-45] graphite/epoxy laminate as shown in Figure. Assume that each lamina has a thickness of 5 mm.
38 Step 3: Find the coordinate of the top and bottom surface of each ply using equation 4.20 The total thickness of the laminate is h = (0.005)(3) = m.The midplane is m from the top and the bottom of the laminate.Ply n:h0 = – mh1 = – mh2 = mh3 = m
39 Step 4: Find three stiffness matrices [A], [B], and [D]